Significance and Use
5.1 Tensile properties determined by this test method are of value for identifying and characterizing materials for control and specification purposes as well as for providing data for research and development studies.
5.2 This test method is intended for use in testing resin-compatible sized glass fiber materials that have been designed specifically for use with certain generic types of plastics. The use of a resin system that is compatible with the reinforcement material under test produces results that are most representative of the actual strength that is available in the material when used as intended in an end item. Premature reinforcement failures occur if the elongation of the resin system is less than that of the reinforcement being tested. It is critical to select a resin system that does not lead to premature reinforcement failure. Use of compatible resin system and complete resin impregnation is recommended to avoid invalid failures and misleading results.
5.3 This test method is useful for testing pretreated specimens for which comparative results are desired. Gage length, gripping system, testing speed, and the resin impregnation ratio of the specimen affects the values obtained by this test method.
1.1 This test method covers the determination of the comparative tensile properties of glass fiber strands, yarns, and rovings in the form of impregnated rod test specimens when tested under defined conditions of pretreatment, temperature, humidity, and tension testing machine speed. This test method is applicable to continuous filament, glass fiber materials that have been coated with a resin compatible sizing. This method is intended for use in quality control and R & D, and is not intended to be used to develop composites design data.
Note 1: This method is technically equivalent to the short method described in ISO 9163.
Note 2: Prime consideration should be given to the use of a polymeric binder that produces specimens that yield the highest consistent values for the glass fiber material under test. Tensile properties vary with specimen preparation, resin impregnation system, and speed and environment of testing. Consider these factors where precise comparative results are desired.
1.2 The values stated in SI units are to be regarded as the standard. The values given in parentheses are for information only.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.